Low Temperature Physical-Chemical Vapor Deposition
of Ti-Si-N-O Barrier Films
Y. C. Ee, a,b,z Z. Chen, a T.-M. Lu, c Z. L. Dong, a and S. B. Law b
School of Materials Science and Engineering, Nanyang Technological University, Singapore 639798
Chartered Semiconductor Manufacturing Limited, Department of Technology and Development,
Center of Integrated Electronics, Rensselaer Polytechnic Institute, Troy, New York 12180, USA
Ti-Si-N-O films were grown by radio frequency reactive magnetron sputtering of a titanium target with nitrogen and silane gases
introduced at a temperature of 40°C. X-ray diffraction and X-ray photoelectron spectroscopy results show that Ti-N, Si-N, Ti-Si,
Ti-O, Si-O, and Si-N-O compounds are formed. High-resolution-transmission-electron-microscopy reveals that the film consists of
Ti-N, Si-N, Ti-Si nanocrystals embedded in an amorphous Ti-O, Si-O, and Si-N-O matrix. This type of microstructure gives rise
to very high stability against copper diffusion under bias temperature stressing BTS compared to binary barrier materials. The
BTS result shows that Ti 24Si 12N 35O 29 film can effectively block copper ion diffusion for up to 200°C at 0.5 MV/cm.
© 2006 The Electrochemical Society. DOI: 10.1149/1.2166510 All rights reserved.
Manuscript submitted September 16, 2005; revised manuscript received November 28, 2005.
Available electronically January 18, 2006.
It is now well recognized that future improvements in the performance
of integrated circuits will depend heavily on improvements
in the efficiency with which circuit elements are interconnected.
Use of the Cu interconnects in microelectronic devices
require development of barrier layers which can effectively prevent
Cu diffusion into dielectric layers and Si substrates under the influence
of electrical and thermal stresses. Extensive work in the deposition
of TiN barrier film by both sputtering 1,2 and chemical vapor
deposition 3,4 have been reported. A common denominator underlying
many of the above references is the columnar structure of TiN,
typically with a 111 or 200 preferred orientation. Such a structure
can lead to short-circuit diffusion paths via grain boundaries and
result in the failure of the devices. With the down-scaling of devices
and more stringent reliability requirements, there is a need for more
effective barrier materials. To this end, a class of refractory, ternary
nitride materials, such as Ti-Si-N, 5 Ta-Si-N, 6 and W-Si-N 7 have
been proposed as candidates for the next generation diffusion barrier
in copper/low-k dielectric back-end-of-line device fabrication. 8,9
One of the advantages of these ternary barrier films is attributed to
the mixed microstructure which consists of nanocrystalline M-N
M = Ti, Ta, W embedded in amorphous matrix Si-N.
The barrier material that we have investigated is Ti-Si-N-O films
which consist of nanocrystals embedded in an amorphous matrix,
but the amorphous matrix in this Ti-Si-N-O film is contributed by
Ti-O, Si-O, and Si-N-O phases rather than the Si-N phase. It exhibits
excellent barrier properties against Cu ion diffusion under biastemperature
In this article, we present a process for low-temperature physicalchemical
vapor deposition of Ti-Si-N-O barrier films. Film composition,
microstructure, and chemical bonding state have been analyzed.
The barrier films showed excellent stability against bias
temperature stressing BTS, which makes them attractive candidates
as future generation barrier materials.
A 630 nm thick plasma enhanced chemical vapor deposition
PECVD SiO 2 layer was first deposited on a p-type silicon substrate
using tetraethyl orthosilicate, SiOC 2H 5 4 and oxygen as precursors.
The deposition temperature was between 350–450°C and the
pressure was 4–6 Torr. This was followed by the deposition of
215 nm Ti-Si-N-O films by radio frequency rf reactive magnetron
sputtering of Ti target in a chamber with a base pressure of 3.75
10 −5 Torr. Processing gases such as silane as a precursor, and
other gases like nitrogen and argon were introduced. The pressure
was maintained at 7.1 10 −3 Torr during the deposition process.
No substrate heating or bias were provided. The substrate tempera-
z E-mail: PA8898695@ntu.edu.sg
Electrochemical and Solid-State Letters, 9 3 G100-G103 2006
1099-0062/2006/93/G100/4/$20.00 © The Electrochemical Society
ture was measured to be 40°C when 300 W rf power was applied to
the titanium target. Silane, nitrogen, and argon gas flow rates were
maintained at 20, 30, and 20 sccm, respectively. Composition was
obtained by Rutherford backscattering spectrometry RBS using a
2.0 MeV 4 He + beam with the 4.0 MV Dynamitron accelerator at the
Ion Beam Laboratory, Department of Physics, University of New
York at Albany.
Phase composition was investigated through X-ray diffraction
XRD using a Shimadzu XRD 6000 diffractometer. The chemical
states of titanium, silicon, and nitrogen were analyzed by X-ray
photoelectron spectroscopy XPS using 1486.71 eV Al K irradiation.
The X-rays and the peak positions were calibrated with respect
to the C 1s peak at 284.44 eV. High resolution transmission electron
microscopy HRTEM was used to characterize the nanostructure of
the films. C–V measurements were made on a HP 4280A 1 MHz
capacitance meter/C–V plotter to study the bias temperature stability
of the Ti-Si-N-O films against Cu ion diffusion. A small ac
signal of 10 mV rms was superposed on the applied dc bias. The
Cu/Ti-Si-N-O/SiO 2/Si capacitors were fabricated on Si wafers secured
by vacuum chucking to an MSI Electronics light shield/hot
chuck and were under nitrogen purge throughout the experiment.
BTS experiments were performed at temperatures ranging from
150–200°C with a bias of 0.5 and 1 MV/cm, and biasing time of
5–90 min. The samples were biased at high temperatures, then water
cooled rapidly down to room temperature with bias on at periodic
intervals for C–V measurements.
The thickness of the Ti-Si-N-O film measured by a surface profiler
was 215 nm. Although the films investigated are too thick to
serve as barrier layers in current devices, in this study we focus on
the microstructure and the presence of oxygen in Ti-Si-N-O layers
and the resulting implication to barrier properties. Investigation of
thinner layers is under investigation. The electrical resistivity for
this barrier film is 3629 cm. According to International Technology
Roadmap for Semiconductor, 2004, 9 when the technology
node reduces from 90 to 65 nm, the required barrier thickness will
reduce from 8 to 4.5 nm. With such an ultrathin barrier, electrons
can tunnel through the barrier film when the current pass through the
copper vias. Thus, electrical resistivity of barrier will not be a major
issue for future interconnects.
The atomic composition of the Ti-Si-N-O films was determined
by Rutherford backscattering spectrometry RBS. Figure 1 shows
the backscattering spectrum of a Ti-Si-N-O/SiO 2/Si sample, indicating
the presence of nitrogen, oxygen, silicon, and titanium. The
film contains 12 atom % of silicon when the silane gas SiH 4 flow
rate was 20 sccm. The corresponding stoichiometric composition
was Ti 24Si 12N 35O 29. XPS measurement shows a similar result, thus
only the composition by RBS is used in the paper. In addition, XPS
4 He +
Figure 1. 2.0 MeV backscattering spectrum of the
Ti-Si-N-O/SiO2/Si sample. Ti-Si-N-O films were deposited at 20 sccm silane
gas flow while the nitrogen gas flow rate and argon gas flow rate were
maintained at 30 and 20 sccm, respectively.
further indicates the simultaneous formation of Ti-N, Si-N, Ti-Si,
Ti-O, Si-O, and Si-N-O bonds when Ti 2p, Si 2p, N 1s, and O 1s
peaks are deconvoluted. The presence of crystal phases, Ti-N, Si-N,
and Ti-Si are further confirmed by XRD as shown in Fig. 2. Oxygen
was detected throughout the thickness of the films. The presence of
oxygen in the prepared barrier films could be due to the high reactivity
of titanium and silicon with residual oxygen and water in the
vacuum chamber. The incorporation of oxygen in TiN or Ti-Si-N
film has been reported by Olowolafe et al., 10 Cheung et al., 11 Lemperiere
et al., 12 Zhang et al., 13 and Shtansky et al. 14 In the work of
Shtansky et al., 14 1–5 atom % of O was found in Ti-Si-N film with
a bias of −250 to 0 V during the deposition process. In the work by
Olowolafe et al., 10 25 atom % of O was obtained in the deposition of
TiN film in a base vacuum of 2 10 −7 Torr without substrate bias.
In the current work, no bias was applied to the substrate in the
preparation of Ti-Si-N-O films with vacuum level of 3.75
10 −5 Torr. We believe that bias will create a concentrated flux of
sputtered species onto the substrate; such a high concentration prevents
oxygen from getting close to the substrate surface due to pres-
Figure 2. XRD measurement of Ti-Si-N-O films at silane gas flow rate of
20 sccm. Ti-N, Si-N, and Ti-Si phases are detected.
Electrochemical and Solid-State Letters, 9 3 G100-G103 2006 G101
sure difference. Without the bias, the oxygen in the chamber has
good access to the film to react with Ti and Si, and resulted Ti-O,
Si-O, and Si-N-O bonds as shown in Fig. 3.
Figure 4 shows the plan view of a high resolution TEM
HRTEM micrograph of the Ti 24Si 12N 35O 29 film. It is observed that
2 to 15 nm crystals were formed with an average crystallite size of
9 nm. Combining XPS one XRD results and lattice spacing measurement
from HRTEM, these nanocrystals are identified as Ti-N,
Si-N, and Ti-Si phases. The remaining Ti-O, Si-O, and Si-N-O compounds
are in an amorphous state.
In the work by Marcadal et al., 8 nanocrystallites of TiN were
reported to be embedded in amorphous Si xN y matrix. In such a
configuration, fast diffusion channels were said to be absent since
there was no percolation via grain boundaries in this microstructure.
Reid et al. 15 also reported the mixed microstructure of Ti-Si-N films,
and the random arrangement of the nanophase of TiN eliminates
straight grain boundary paths associated with most columnar TiN
films. In addition, the integranular silicon components may be
viewed as severely stuffing the grain boundaries of TiN, and thus
improved the barrier performance. Similar to the work by Marcadal
et al., 8 the current study also produced nanocrystals embedded in an
amorphous matrix. But the amorphous phases were not caused by
silicon nitride any more. Si 3N 4 was in crystalline form while the Si
and Ti oxides were in an amorphous form. Apparently the formation
of the oxides has significantly reduced the vitrification temperature
of silicon nitride.
The barrier performance of Ti 24Si 12N 35O 29 films against the Cu
ions diffusion was evaluated through BTS testing. In the work of
Mallikarjunan et al., 16 copper was known to drift into PECVD oxide.
On the other hand, when a metal insulator semiconductor MIS
capacitor Cu/Ti 24Si 12N 35O 29/PECVD SiO 2/Si was bias-temperature
stressed at 150°C and 1 MV/cm for 5, 15, 30, 60, and 90 min, no
flatband voltage shift was observed. In order to explore the electrical
stability limit of the Ti 24Si 12N 35O 29 film against Cu ion diffusion,
the sample was further bias-temperature stressed at the BTS conditions
of 200°C and 0.5 MV/cm. Still there was no flatband voltage
shift as shown in Fig. 5. The large negative flatband voltage that
exists in the as-annealed sample is due to the presence of interface
states at Ti-Si-N-O/SiO 2 and SiO 2/Si interfaces. These interface
states may be produced during processing of the films and can be
reduced by annealing at 300°C in Ar−3% H 2 before BTS testing.
With this pretreatment, the initial flatband voltage is −5 V. This
indicates that the film is stable under these test conditions, which
can satisfy the BTS requirement for barrier materials. Typical computer
chip operating conditions is 200°C and 0.1 MV/cm. 17
So far there have been limited reports about BTS stability for
ternary barrier materials. Smith et al. reported BTS results at 50 V
and 200°C on 10 nm thick MOCVD TiSi xN y samples. They found
that the MTTF of an MOCVD Ti 23Si 14N 45O 3C 3H 12 sample deposited
at 400°C was approximately 10–100 times better than that of
PVD TiN. 18 In general, the stability result depends on the materials,
bias, testing temperature, and duration. In the work by Kizil and
Steinbrüchel, 19 90% barrier failure was found for amorphous TiN
after 90 min BTS at 150°C under 2 MV/cm. Although amorphous
TaN performed better than the TiN, 40% barrier failure still could be
observed after the same BTS condition. In addition, all barriers fail
more rapidly at the higher temperature, indicating that BTS stability
is very sensitive to temperature rise. Based on these limited reports
and our current work, ternary and quaternary barriers seem to perform
better than binary system.
The reasons for the good barrier performance of the current Ti-
Si-N-O system are suggested as follows: i stuffing of oxygen at the
boundary of nanocrystals. In the work by McArthur et al., 20 the
improved Ti-Si-N barrier properties were believed to be due to the
grain boundary stuffing of the crystallized TiN with oxygen. In our
Ti-Si-N-O films, Si-N nanocrystals are formed, and these crystals
can readily accommodate other atoms such as O. 21 Thus it is believed
that O resides at the boundaries of both Ti-N and Si-N, making
the diffusion of Cu ions through the grain boundaries more
Electrochemical and Solid-State Letters, 9 3 G100-G103 2006
difficult. ii The presence of an amorphous phase reduces the density
of grain boundaries. Marcadal et al., 8 Eisenbraun et al., 22 Joseph
et al., 23 Muira et al., 24 and No et al., 25 reported that the improved
barrier properties of Ti-Si-N were related to the formation of an
amorphous phase in the Ti-Si-N film. In these reports, the amorphous
matrix consisted of the Si-N phase. But the amorphous matrix
in our Ti-Si-N-O film is formed by Ti-O, Si-O, and Si-N-O phases.
These Ti-O and Si-O bonds play an important role in the barrier
performance as discussed next. iii Thermodynamic data 26 shows
that the enthalpies of formation H f of Ti-O and Si-O are
Figure 4. High resolution TEM reveals that the film consists of nanocrystals
embedded in an amorphous matrix.
Figure 3. XPS analysis shows that oxygen
bonded to titanium, silicon, and nitrogen
forming titanium oxide, silicon oxide
and silicon oxynitride when O 1s peak is
−944.746 and −910.866 kJ/mol, respectively, at 300 K, compared
to that of −156.057 kJ/mol for Cu-O. As reported by Mallikarjunan
et al. 27 metals ionize when in contact with interfacial oxygen. Ionized
copper may then diffuse into the dielectric under applied bias.
The tendency for such a diffusion critically depends on the formation
of the Cu-O bond. When Ti-O and Si-O are already present in
the film before Cu deposition, the energy needed to break the Ti-O
and Si-O bonds to make O available for the Cu-O bond is much
higher based on the thermodynamic data. Thus the formation of
Cu-O is relatively difficult and the ionization tendency of Cu is
reduced with the presence of Ti-O and Si-O compounds.
In summary, a physical-chemical vapor deposition process for
Ti-Si-N-O barrier was developed at 40°C. Ti-N, Si-N, and Ti-Si
nanocrystals are formed and embedded in Ti-O, Si-O, and Si-N-O
amorphous matrix. With this type of mixed structure, a very good
electrical stability of Ti-Si-N-O film against copper ion diffusion is
achieved, and it is able to prevent copper ions drifting into subsequent
dielectric layers even when bias temperature stressed at
Figure 5. C–V plots of the MIS capacitor Cu/Ti 24Si 12N 35O 29/PECVD
SiO 2/Si that bias temperature stressed at 200°C and 0.5 MV/cm. No flatband
voltage shift is observed.
200°C and 0.5 MV/cm. These characteristics make Ti-Si-N-O an
attractive candidate for future ultralarge scale integration diffusion
Nanyang Technological University assisted in meeting the publication
costs of this article.
1. N. Kumar, J. T. McGinn, K. Pourrezaei, B. Lee, and E. C. Douglas, J. Vac. Sci.
Technol. A, 6, 1602 1988.
2. S. Kanamori, Thin Solid Films, 136, 195 1986.
3. N. Yuokoyama, K. Hinode, and Y. Homma, J. Electrochem. Soc., 138, 190 1991.
4. K. Ishihara, K. Yamazaki, and H. Hamada, Jpn. J. Appl. Phys., Part 1, 29, 2103
5. P. M. Smith and J. S. Custer, Appl. Phys. Lett., 70, 31161997.
6. Y.-J. Lee, B.-S. Suh, M. S. Kwon, and C.-O. Park, J. Appl. Phys., 85, 1927 1999.
7. J. S. Reid, E. Kolawa, C. M. Garland, M.-A. Nicolet, F. Cardone, D. Gupta, and R.
P. Ruiz, J. Appl. Phys., 79, 1109 1996.
8. C. Marcadal, M. Eizenberg, A. Yoon, and L. Chen, J. Electrochem. Soc., 149, C52
9. International Technology Roadmap for Semiconductors, Semiconductor Industry
Association, San Jose, CA 2004.
10. J. O. Olowolafe, J. Li, J. W. Mayer, and E. G. Colgan, Appl. Phys. Lett., 58, 469
11. N. W. Cheung, H. von Seefeld, and M.-A. Nicolet, in Thin Film Interfaces and
Interactions, J. E. E. Baglin and J. M. Poate, Editors, PV 80-2, p. 323, The Electrochemical
Society Proceedings Series, Princeton, NJ 1980.
12. G. Lemperiere and J. M. Poitevin, Thin Solid Films, 111, 339 1984.
Electrochemical and Solid-State Letters, 9 3 G100-G103 2006 G103
13. C. H. Zhang, Z.-J. Liu, K. Y. Li, Y. G. Shen, and J. B. Luo, J. Appl. Phys., 95, 1460
14. D. V. Shtansky, I. V. Lyasotsky, N. B. D’yakonova, F. V. Kiryukhantsev-Korneev,
S. A. Kulinich, E. A. Levashov, and J. J. Moore, Surf. Coat. Technol., 182, 204
15. J. S. Reid, X. Sun, E. Kolawa, and M.-A. Nicolet, IEEE Electron Device Lett., 15,
16. A. Mallikarjunan, S. P. Murarka, C. Steinbruchel, A. Kumar, and H. Bahkru, J.
Electrochem. Soc., 147, 3502 2000.
17. A. E. Kaloyeros and E. Eisenbraun, Annu. Rev. Mater. Sci., 30, 363 2000.
18. P. Smith, J. Custer, R. Jones, A. Maverick, and D. Roberts, in Advanced Metallization
and Interconnect Systems for ULSI Applications, p. 249, Mater. Res. Soc.
Symp. Proc., Pittsburgh, PA 1996.
19. H. Kizil and C. Steinbrüchel, Thin Solid Films, 449, 158 2004.
20. W. F. McArthur, K. M. Ring, and K. L. Kavanagh, Final Report 1997–98 for
MICRO Project No. 97-078 1998.
21. H. O. Pierson, Handbook of Refractory Carbides and Nitrides: Properties, Characteristics,
Processing, and Applications, Noyes Publications, Park Ridge, NJ
22. E. Eisenbraun, A. Upham, R. Dash, W. X. Zeng, J. Hoefnagels, S. Lane, D. Anjum,
K. Dovidenko, A. Kaloyeros, B. Arkles, and J. J. Sullivan, J. Vac. Sci. Technol. B,
18, 2011 2000.
23. S. Joseph, M. Eizenberg, C. Marcadal, and L. Chen, J. Vac. Sci. Technol. B, 20,
24. Y. Miura and S. Fujieda, J. Appl. Phys., 81, 6476 1997.
25. J.-T. No, J.-H. O, and C. M. Lee, Mater. Chem. Phys., 63, 442000.
26. I. Barin, F. Sauert, E. Schultze-Rhonhof, and W. S. Sheng, Thermochemical Data
of Pure Substances, 2nd ed., VCA, Weinheim 1993.
27. A. Mallikarjunan, S. P. Murarka, and T.-M. Lu, Appl. Phys. Lett., 79, 1855 2001.